ERRATUM

M. P. H. Thurlings, E. Frikkee, and H. W. de Wijn, “Spin-wave analysis in the two-dimensional antiferromagnet K_2FeF_4. I. Neutron scattering,” Phys. Rev. B 25, 4750 (1982)

Table I should read:

Table I. Relative intensities of (10l) magnetic Bragg peaks at 4.2 K for various geometries, specified by the orientation of the spins (relative to the magnetic until cell) and the order within sheets spanned by the spin orientation and the c axis. The neutron wavelength is 1.473 Å.

Orientation Sheets (100) (101) (102) (103) (104)

[100], [010]

Ferromagnetic 1.00 0.15 0.67 0.30 0.32 Antiferromagnetic 0.00 0.89 0.30 0.47 0.24

[110], [110] (Anti)ferromagnetic 0.50 0.52 0.49 0.39 0.28

[001] 1.00 0.74 0.37 0.16 0.07

Experiment 1.0 0.15 1.0 0.32 0.5

The corrections do not alter the conclusion that the spins are oriented along the magnetic axes in ferromagnetic sheets.